www.nature.com/scientificreports
OPEN
Received: 8 May 2017 Accepted: 9 August 2017 Published: xx xx xxxx
Highly tunable timereversalinvariant topological superconductivity in topological insulator thin films Fariborz Parhizgar1,2 & Annica M. BlackSchaffer2 We study timereversalinvariant topological superconductivity in topological insulator (TI) thin films including both intra and intersurface pairing. We find a nontrivial topology for multiple different configurations. For intrasurface pairing a πphase difference between the intrasurface pairing states is required. We show that in this case the resulting topological phase is highly tunable by both an applied electric field and varied chemical potential. For spinsinglet intersurface pairing, a signchanging tunnel coupling present in many TI thin films is needed, and again, the topology can be tuned by electric field or doping. Notably, we find that the required intersurface pairing strength for achieving nontrivial topology can still be subdominant compared to the intrasurface pairing. Finally, for spintriplet intersurface pairing we prove that the superconducting state is always topological nontrivial. We show that thin films of Cudoped Bi2Se3 will likely host such spintriplet intersurface pairing. Taken together, these results show that timereversalinvariant topological superconductivity is common in superconducting TI thin films and that the topological phase and its Kramers pair of Majorana edge modes is highly tunable with an applied electric field and varied chemical potential. Topology in condensed matter systems has received a massive amount of interest in recent years. Starting with the discovery of topological insulators (TIs)1–4, where nontrivial topology of the bulk band structure creates surface states with a Diracspectrum crossing the bulk band gap, topology is now also applied widely in the discussion of properties of superconductors and semimetals5–8. In topological superconductors the zeroenergy surface states are particularly intriguing as they are Majorana modes, due to their equal electron and hole characteristics9–12. The nonAbelian statistics of Majorana zeromodes makes topological superconductors very promising for topological quantum computation13–15. Many topological superconductors explicitly break timereversal symmetry. This is usually achieved by magnetic field or impurities, which together with Rashba spinorbit coupling and superconductivity can give nontrivial topology16–23. A close alternative is superconducting TI surfaces, where Majorana modes appear in vortex cores or at ferromagnetic interfaces, again requiring magnetic fields24–28. However, timereversalinvariant superconductors can also be topologically nontrivial, where instead the surface spectrum consists of a Kramers pair of helical Majorana modes29. Despite the doubling of the Majorana modes, nonAbelian operations have still been demonstrated in these systems30. Since superconductivity is generally very sensitive to magnetic fields, timereversalinvariant systems have a very natural advantage in terms of stability of the superconducting phase. Proposals for timereversalinvariant superconductors have mainly been based on multichannel systems, since noninteracting singlechannel systems with conventional swave superconductivity cannot be topological31. For example, multiband/orbital systems and s±wave ironbased superconductors have been shown to be able to host a nontrivial phase32–34. Double wire systems with Rashba spinorbit coupling have also been studied, where a πphase difference of the superconducting order parameter between the two wires35, or a strong interwire pairing36–39 have been shown to give nontrivial topology. Similar topological interwire superconductivity has been found using two 1D edges from two independent 2D TIs40. A 1D extended Hubbard chain also has been shown to 1
School of Physics, Institute for Research in Fundamental Sciences (IPM), Tehran, 193955531, Iran. 2Department of Physics and Astronomy, Uppsala University, P.O. Box 516, S751 20, Uppsala, Sweden. Correspondence and requests for materials should be addressed to F.P. (email:
[email protected]) or A.M.B.S. (email: annica.
[email protected]) Scientific REPOrTS  7: 9817  DOI:10.1038/s4159801710510y
1
www.nature.com/scientificreports/

Figure 1. Two different schematic setups for proximityinduced superconductivity in 3D TI thin films. Green area represents the TI thin film with its two surfaces (dark green), t(k) the tunneling, and 2V an applied electrostatic potential. Yellow parts are swave superconductors, where the superconducting phase can be controlled by the magnetic flux 2ϕ (a) or an asymmetry can be induced in the intrasurface pairing strength (b). Depicted are both intra (left) and intersurface (right) Cooper pairs. vF (105 ms−1)
t0 (eV)
t1 (eVÅ2)
2 QLs
4.71
0.125
21.8
3 QLs
4.81
0.069
18.0
4 QLs
4.48
0.035
10.0
Table 1. Parameters in the Hamiltonian Eq. (1) for Bi2Se3 TI thin films, extracted by fitting the dispersion relation with ARPES data (adopted from ref. 45). support topological superconductivity in the presence of both singlet and triplet pairing41. In addition, a πphase difference has been shown to give a nontrivial topology in a simple model for unbiased TI thin films42 and by introducing random magnetic moments between a superconductor and a TI surface43. Similar criteria have been found in double layer Rashba materials with strong interactions44. However, all these systems have shown zero or very limited tunability of the topological phase by experimentally controllable parameters, which both limit applications and possibilities to detect nontrivial topological phases. In this work we study conventional swave superconductivity in realistic models of superconductivity in threedimensional (3D) TI thin films. For TI films thinner than 6 quintuple layers (QL), an energy gap opens in the surface states due to intersurface tunneling45. However, sufficient doping produces a finite density of states at the Fermi level, such that thin films can easily enter a superconducting phase either by proximity to external superconductors27, 46, or possibly by an intrinsic mechanism47–53. To allow for the most general situation we consider both swave intrasurface pairing and intersurface pairing, since intersurface pairing has been shown to be present in proximityinduced superconducting thin films through crossed Andreev reflection54, 55 and from a direct proximity effect56. We show that intrasurface pairing can lead to a topologically nontrivial state when there is a πphase difference between the two surface pairing terms. Further, spintriplet intersurface pairing is odd in surface index, which we show always result in a topologically nontrivial state. For nontrivial topology with spinsinglet intersurface pairing, the thin film tunneling needs to change sign with momentum, which is very common in TI thin films. Most importantly, in all cases the topological phase is highly tunable with an applied electric field or by varying the chemical potential. This allows for direct tuning of timereversalinvariant topological superconductivity and its associated Kramers pair of Majorana edge modes in TI thin films. With proximityinduced superconductivity already established in 3D TI thin films and intrinsic superconductivity found in several TIs, our results should have direct experimental relevance.
Model Hamiltonian
Figure 1 shows two different schematics of the system we study. The TI thin film (green) is acting like a bilayer material with tunneling t(k) between its two surfaces and is in proximity to a conventional superconductor (yellow). We also allow for an electrostatic potential difference 2V between the two surfaces, which causes a structure inversion asymmetry. The flux ϕ in Fig. 1(a) induces a phase difference between the pairing amplitudes in the two surfaces, but at ϕ = π timereversal symmetry is still preserved35. In the setup in Fig. 1(b) the intrasurface pairing is clearly different between the two surfaces. Intersurface pairing can be prominent in both setups, and particularly in (b)56. The effective lowenergy Hamiltonian of the 3D TI thin film can be written as57, 58: h(k) = vF(k ⋅ σ ) ⊗ τz + t(k)σ0 ⊗ τx + Vσ0 ⊗ τz − µσ0 ⊗ τ0.
(1)
Here k = (kx, ky) with k = k and vF is the Fermi velocity, while σ and τ are Pauli matrices in spin and surface space, respectively. The intersurface tunneling t(k) in TI thin films is of the form t0 − t1k2 45. Values for the intrinsic parameters for thin films of the prototypical TI Bi2Se3 are given in Table 1. Due to a finite t0, intrinsic Bi2Se3 thin films have a completely gapped spectrum. Finally, tunable parameters are both the electrostatic potential V, by applying an electric field as a gate voltage, and the chemical potential μ, which is adjustable by e.g. chemical doping. In order to achieve a sustainable superconducting state we assume a finite doping, such that the Fermi level is located inside the conduction band. The normal state band dispersion of the Hamiltonian in Eq. (1) is given by ε(k) = ± t(k)2 + (vFk ± V )2 . By equating this energy to the chemical potential we find two different Fermi wavevectors kF±, which produce two Scientific REPOrTS  7: 9817  DOI:10.1038/s4159801710510y
2
www.nature.com/scientificreports/
Figure 2. Schematic figure of the band dispersion of a TI thin film in the normal state. Due to finite tunneling between the two surfaces, a gap occurs in the band dispersion. The potential V gives rise to a Rashba splitting between the bands, such that at a finite chemical potential two Fermi circles with radii kF− and kF+ appears.
concentric Fermi level circles centered around the Brillouin zone center k = 0. Figure 2 shows a schematic of the band dispersion of a TI thin film. As seen, a finite potential V causes a Rashba splitting of the bands, which is the origin of the existence of the two Fermi circles with radii kF±. Note that for all small to moderately large μ and V, all the relevant lowenergy physics will be closely centered around the Brillouin zone center. Superconductivity in TIs can be either intrinsic47–53, 59, 60 or induced by proximity to an external superconductor27, 46. To allow for a general situation, we consider both Cooper pairs formed within each surface, intrasurface pairing Δ1 and Δ2, and between the two surfaces, intersurface pairing Δ12. Note that intersurface pairing can be quite prominent in setups such as Fig. 1(b)56. Since higher momentum states are much more fragile in the presence of any disorder in systems with timereversal symmetry according to Anderson’s theorem61, we focus only on swave superconducting symmetries even when studying clean systems. It is also worth mentioning that an swave nature of the intrinsic superconductivity in CuxBi2Se3 has been confirmed experimentally62. This results in the total order parameter in the surface basis being s t ∆1 ∆12 + ∆12 , ˆ = ∆ ∆s − ∆t ∆ 12 12 2
(2)
where the intrasurface pairing is necessarily spinsinglet, while intersurface pairing can be either spinsinglet (s) or triplet (t), depending on the parity in surface index being even or odd, respectively. Finally, the total BdG Hamiltonian of the system, written in Nambu space, (ψk† ψ−Tk), is h(k) ˆ ∆ † † † † † H (k) = † where ψ k = (ck,1 ↑c k,1 ↓c k,2 ↑c k,2 ↓) . ∆ ˆ −h( − k)T
(3)
Results
Topological order. For a timereversalinvariant system we can rotate the BdG Hamiltonian in Eq. (3) and
write it in the basis of
Ψk =
† T 1 ψk − iTˆ (ψ−k) . 2 ψk + iTˆ (ψ−†k)T
(4)
This results in 0 h(k) + iTˆ ∆† H (k) = , h(k) − iTˆ ∆† 0
(5)
where Tˆ = τ0 ⊗ iσyκ is the timereversal matrix, with κ the complex conjugation operator. Following ref. 63 we now define the matrix element δn(k) = ψn(k) Tˆ ∆† ψn(k) ,
(6)
where ψn(k)〉 is the wave function of the nth band of the normal state Hamiltonian h(k). In the weak pairing limit it is only the electrons very near the Fermi surface that are important for superconductivity, and the above equation can then be calculated at the two Fermi wavevectors kF± of the TI thin film. Applying this expression in 2D, Scientific REPOrTS  7: 9817  DOI:10.1038/s4159801710510y
3
www.nature.com/scientificreports/
Figure 3. Topological phase diagram for Bi2Se3 TI thin films for finite intrasurface pairing in the plane of (a) (−Δ1, Δ2) and (b–d) (V, μ). In (a) dashed (3, 4 QLs) and dotted (2 QLs) lines display the topological criterion based on δn in Eq. (7), while solid red lines show the gap closing for the full Hamiltonian Eq. (3) for 2 QLs. Here μ = 0.1 eV and V = 0.1 eV. In (b–d) Δ1 = −Δ2 for 2–4 QL thick films with nontrivial phase in orange.
the topological order can be classified by the expression N2D = Πn(sgn(δn))mn, where mn is the number of timereversalinvariant points enclosed by the normal state Fermi surface(s). Since the only timereversal symmetric point enclosed by the two Fermi circles is k = (0, 0), we find mn = 1. Staying within the weakpairing limit, δn(k) is only nonzero close to the Fermi surface and for a fullygapped superconductor it remains finite on all Fermi surfaces, which makes the sign of δn(k) a good topological number. After some calculations we also obtain the normalized wave functions corresponding to the two bands crossing the Fermi surface as ψn T =
θn iφ θn θn iφ 1 θn cos , ncos e k, sin , n sin e k , 2 2 2 2 2
where n = ±1 indicates the two different conduction bands and φk is the polar angle of the momentum. We have also defined the new variable θn, such that sin(θn) = t(kFn)/ (vFkFn + nV )2 + t(kFn)2 . Using the above wave functions, together with Eqs (2) and (6), we arrive at δn =
cos2
( ) ∆ + ∆ tan θ + 2∆
2
θn 2
1
2
2
n
2
θn s 12 tan , 2
(7)
for a spinsinglet swave superconducting state in a TI thin film. Note however that the spintriplet intersurface pairing is absent in this expression since it is odd under the surface index and thus necessarily gives a zero contribution in Eq. (6).
Intrasurface pairing. We first consider the case of zero or negligible intersurface pairing and focus on only finite intrasurface orders Δi. We assume that Δi is either produced by an intrinsic mechanism or by proximity effect to a conventional superconductor, in both cases resulting in spinsinglet swave symmetry. The setup in Fig. 1(a) for proximityinduced superconductivity allows for separately tuning the superconducting phases induced in the two surfaces of the TI thin film by controlling the magnetic flux. The two order parameter amplitudes can also be different by modifying the coupling between the TI thin film and the superconductor. From Eq. (7) it is clear that if the superconducting orders have the same sign, Δ1Δ2 > 0, then δn always has the same sign for all bands. Thus, there exists no nontrivial topological phase if there is no phase difference between the superconducting states in the two surfaces. Limiting ourselves to timereversalinvariant superconductivity, a πshift is also allowed between the two superconducting states. This can clearly be achievable by tuning the flux in Fig. 1(a). Alternatively, as has recently been found in 1D systems64, 65, possibly also driven by electronelectron interactions. In this latter case meanfield theory as well as density matrix renormalization group calculations were used to show that repulsive electronelectron interaction can result in a πphase shift between two parallell systems. Moreover, intrinsically πshifted pairing terms have also recently been studied in general twoband systems33. Taken together, it is therefore relevant to consider this case also for TI thin films. For the situation Δ1Δ2 ∆1 = ∆2 in order to reach a nontrivial state. Near the limit Δi = 0, the sign of δn is simply equal to the sign of t(kFn) on each Fermi surface. Such dominating intersurface pairing can easily be a consequence of intrinsic pairing. It has also been found for proximityinduced superconductivity in double 1D wire systems with strong electronelectron interactions, where the repulsive interaction heavily suppresses intrawire pairing, while interwire pairing is significantly less affected36–39, 66–68. Also in 2D layer systems, dominating interlayer pairing has recently been studied44, 69. In addition, it has recently been found that screening has a stronger effect on intralayer properties than on interlayer ones in double layer graphene systems70. Together these results clearly validates studying also the strong intersurface pairing regime. Note though that we do not explicitly include the effects of electronelectron interactions. However, since the derived conditions for nontrivial topology are independent on the size of the individual pairing amplitudes, any band or pairing renormalizations arising from interaction effects are actually automatically included. Thus, it is possible to study also this regime within our framework. In Fig. 5 we plot the topological phase of a 3 QL Bi2Se3 thin film for finite intersurface pairing with different intrasurface contributions as function of the two tunable parameters V and μ when Δ1 = Δ2. This setup is expected for a superconductor coupling equally well to both surfaces. As the intrasurface pairing approach the intersurface pairing, the nontrivial topological region (purple) shrinks, but a large nontrivial region is present even for substantially large intrasurface pairing amplitudes. Note that these results are not dependent on the actual amplitudes of the different superconducting order parameters, but only on their ratios. Scientific REPOrTS  7: 9817  DOI:10.1038/s4159801710510y
5
www.nature.com/scientificreports/
Figure 5. Topological phase diagram for a 3 QL Bi2Se3 TI thin film for finite spinsinglet intersurface pairing s s in the plane of (V, μ) when (a) Δ1 = Δ2 = 0, (b) ∆1∆2 = 0.3∆12 , (c) ∆1 = ∆2 = 0.6∆12 , and (d) s . ∆1 = ∆2 = 0.9∆12
Figure 6. Topological phase diagram for a 3 QL Bi2Se3 TI thin film for chemical potentials (a) μ = 0.1 eV and s (b) μ = 0.2 eV in the plane of (V , ∆12 ) when the intrasurface pairing is highly assymmetric, here Δ1 = 5Δ2.
Alternatively to Fig. 5 we also consider a superconductor proximitycoupled to only the first TI surface, as in Fig. 1(b). In the ultrathin limit, earlier results have found both finite intrasurface pairing in both surfaces, albeit ∆1 ∆2, and also significant intersurface pairing56. In Fig. 6 we show the topological phase diagram in the s plane of V and ∆12 /∆1 for a fixed typical value of Δ1 = 5Δ2 and two different chemical potentials. The results s clearly show that a nontrivial phase is possible for intersurface order parameter ∆12 notably smaller than Δ1, and that again, the results is highly tunable with V and μ. The clear dependence on the size of the intersurface pairing is somewhat reminiscent to a 1D double Rashba wire system, where topological superconductivity has been found for dominating interwire pairing36. However, note that the topology of TI thin films is not only dependent to this ratio of the pairing amplitudes, but also very sensitive to the sign of the tunneling function t(k) on each Fermi surface. Since this t(kFn) can very readily be tuned by both chemical doping μ and electric potential V, it leads to topology being easily controllable for TI thin films, in contrast to the 1D systems studied previously.
Intersurface spintriplet pairing. Finally we also investigate spintriplet intersurface pairing. A finite
t always gives zero contribution to Eq. (6) since it is odd under the surface spintriplet intersurface pairing ∆12 index, and can thus not be investigated within the above framework. Instead, we make use of previous work on the possible topological phases in the bulk superconducting state in Cudoped Bi2Se3, which is one of the most studied superconducting TIs47–53, 59, 60. Using the lattice symmetries of the centrosymmetric bulk Bi2Se3, the superconducting pair amplitudes in CuxBi2Se3 have been analyzed in terms of their orbital structure, divided into intraorbital spinsinglet and interorbital spinsinglet and triplet states59, 60. It was shown that a fully gapped timereversalinvariant topological superconducting state always exists in this centrosymmetric material for an odd interorbital order parameter, which is necessarily in a spintriplet state59. For the purpose of thin films, we first assume that the thin film limit of CuxBi2Se3 is given by the Hamiltonian Eq. (1) with only a dopinginduced shift of the chemical potential. This is very reasonable since the bulk band dispersion has experimentally been shown to not vary significantly with Cudoping47, 48. Moreover, the upper surface of a TI thin film is almost exclusively composed of one orbital, while the states on the opposite surface come from the other orbital71. Thus we can generalize the bulk results based on orbital parity59 and apply them to the surface parity of a TI thin film. Using this line of argument, we directly find a fully gapped nontrivial topologt ical phase for odd intersurface spintriplet superconducting pairing ∆12 in a TI thin film. Importantly, this directly implicates that thin films of Cudoped Bi2Se3 will have strong dominating spintriplet intersurface pairing, since recent results strongly suggests that the bulk is in an odd interorbital pairing state52, 60. Ultrathin films of Cudoped Bi2Se3, or similarly intrinsic superconducting TIs, are thus a very strong candidate for intersurface pairing forming a 2D topological state with a Kramers pair of helical Majorana 1D edge states. This state is not tunable solely by chemical potential, but applying an electrostatic potential V breaks the structure inversion
Scientific REPOrTS  7: 9817  DOI:10.1038/s4159801710510y
6
www.nature.com/scientificreports/ symmetry, which technically invalidates the above proof of a nontrivial topological state. By numerically studying the energy dispersion of TI thin film nanoribbons, we find that the topologically protected zeroenergy edge states actually prevail to moderately high V, but that the topology becomes trivial above a critical V.
Conclusion
We have investigated the possibilities for timereversalinvariant topological superconductivity in 3D TI thin films. For pure intrasurface pairing we show that topological superconductivity requires the order parameters to have different signs on the two different surfaces. Within this regime, the topology is highly tunable by both doping and electric field. Including strong intersurface pairing alters the criteria for nontrivial topology. For spinsinglet intersurface pairing, nontrivial topology requires the intersurface tunneling to change sign with momentum, a feature very special to TI thin films and highly tunable. Notably, when the intrasurface pairing is asymmetric, for example due to superconducting proximity effect primarily to only one surface, the nontrivial state is reached even for intersurface pairing subdominant compared to the intrasurface pairing. For spintriplet intersurface pairing we prove that the superconducting state is always nontrivial, since it is necessarily odd in the surface index. We also show that the recently suggested odd interorbital pairing state in bulk Cudoped Bi2Se352, 60 results in dominating spintriplet intersurface pairing and thus a nontrivial topological state in TI thin films. These results show that multiple different topological states can exists in superconducting TI thin films. Moreover, the topology is most often highly dependent on the applied electric field and chemical potential, which opens for exciting prospects of insitu tuning of timereversal invariant topological superconductivity and its associated Kramers pair of Majorana edge modes in TI thin films. These results do not only generalize earlier results for double 1D wires to the case of higher spatial dimensions, but importantly shows that the 3D TI thin films offers much more tunability and control of the topological phases. During the final stages of completion of this work, ref. 72. appeared, which treats TI thin films but only includes intrasurface pairing. The results in this limit are similar to ours.
References
1. Kane, C. L. & Mele, E. J. Z2 topological order and the quantum spin hall effect. Phys. Rev. Lett. 95, 146802 (2005). 2. Bernevig, B. A., Hughes, T. L. & Zhang, S.C. Quantum spin hall effect and topological phase transition in hgte quantum wells. Science 314, 1757–1761 (2006). 3. König, M. et al. Quantum spin hall insulator state in hgte quantum wells. Science 318, 766–770 (2007). 4. Hsieh, D. et al. A topological dirac insulator in a quantum spin hall phase. Nature 452, 970–974 (2008). 5. Hasan, M. Z. & Kane, C. L. Colloquium. Rev. Mod. Phys. 82, 3045–3067 (2010). 6. Qi, X.L. & Zhang, S.C. Topological insulators and superconductors. Rev. Mod. Phys. 83, 1057–1110 (2011). 7. Wehling, T., BlackSchaffer, A. & Balatsky, A. Dirac materials. Adv. Phys. 63, 1–76 (2014). 8. Bansil, A., Lin, H. & Das, T. Colloquium. Rev. Mod. Phys. 88, 021004 (2016). 9. Majorana, E. Teoria simmetrica dell’elettrone e del positrone. Il Nuovo Cimento (1924–1942) 14, 171 (1937). 10. Kitaev, A. Y. Unpaired majorana fermions in quantum wires. PhysicsUspekhi 44, 131 (2001). 11. Beenakker, C. Search for majorana fermions in superconductors. Annu. Rev. Condens. Matter Phys. 4, 113–136 (2013). 12. Leijnse, M. & Flensberg, K. Introduction to topological superconductivity and majorana fermions. Semicond. Sci. Technol. 27, 124003 (2012). 13. Ivanov, D. A. Nonabelian statistics of halfquantum vortices in pwave superconductors. Phys. Rev. Lett. 86, 268–271 (2001). 14. Nayak, C., Simon, S. H., Stern, A., Freedman, M. & Das Sarma, S. Nonabelian anyons and topological quantum computation. Rev. Mod. Phys. 80, 1083–1159 (2008). 15. Das Sarma, S., Freedman, M. & Nayak, C. Majorana zero modes and topological quantum computation. Npj Quantum Information 1 (2015). 16. Sau, J. D., Lutchyn, R. M., Tewari, S. & Das Sarma, S. Generic new platform for topological quantum computation using semiconductor heterostructures. Phys. Rev. Lett. 104, 040502 (2010). 17. Lutchyn, R. M., Sau, J. D. & Das Sarma, S. Majorana fermions and a topological phase transition in semiconductorsuperconductor heterostructures. Phys. Rev. Lett. 105, 077001 (2010). 18. Oreg, Y., Refael, G. & von Oppen, F. Helical liquids and majorana bound states in quantum wires. Phys. Rev. Lett. 105, 177002 (2010). 19. BlackSchaffer, A. M. & Linder, J. Majorana fermions in spinorbitcoupled ferromagnetic josephson junctions. Phys. Rev. B 84, 180509 (2011). 20. Choy, T.P., Edge, J. M., Akhmerov, A. R. & Beenakker, C. W. J. Majorana fermions emerging from magnetic nanoparticles on a superconductor without spinorbit coupling. Phys. Rev. B 84, 195442 (2011). 21. Mourik, V. et al. Signatures of majorana fermions in hybrid superconductorsemiconductor nanowire devices. Science 336, 1003–1007 (2012). 22. NadjPerge, S., Drozdov, I. K., Bernevig, B. A. & Yazdani, A. Proposal for realizing majorana fermions in chains of magnetic atoms on a superconductor. Phys. Rev. B 88, 020407 (2013). 23. NadjPerge, S. et al. Observation of majorana fermions in ferromagnetic atomic chains on a superconductor. Science 346, 602–607 (2014). 24. Fu, L. & Kane, C. L. Superconducting proximity effect and majorana fermions at the surface of a topological insulator. Phys. Rev. Lett. 100, 096407 (2008). 25. Fu, L. & Kane, C. L. Josephson current and noise at a superconductor/quantumspinhallinsulator/superconductor junction. Phys. Rev. B 79, 161408 (2009). 26. BlackSchaffer, A. M. & Linder, J. Magnetization dynamics and majorana fermions in ferromagnetic josephson junctions along the quantum spin hall edge. Phys. Rev. B 83, 220511 (2011). 27. Wang, M.X. et al. The coexistence of superconductivity and topological order in the bi2se3 thin films. Science 336, 52–55 (2012). 28. Xu, J.P. et al. Experimental detection of a majorana mode in the core of a magnetic vortex inside a topological insulatorsuperconductor bi2te3/nbse2 heterostructure. Phys. Rev. Lett. 114, 017001 (2015). 29. Qi, X.L., Hughes, T. L., Raghu, S. & Zhang, S.C. Timereversalinvariant topological superconductors and superfluids in two and three dimensions. Phys. Rev. Lett. 102, 187001 (2009). 30. Liu, X.J., Wong, C. L. M. & Law, K. T. Nonabelian majorana doublets in timereversalinvariant topological superconductors. Phys. Rev. X 4, 021018 (2014). 31. Haim, A., Berg, E., Flensberg, K. & Oreg, Y. Nogo theorem for a timereversal invariant topological phase in noninteracting systems coupled to conventional superconductors. Phys. Rev. B 94, 161110 (2016). 32. Zhang, F., Kane, C. L. & Mele, E. J. Timereversalinvariant topological superconductivity and majorana kramers pairs. Phys. Rev. Lett. 111, 056402 (2013).
Scientific REPOrTS  7: 9817  DOI:10.1038/s4159801710510y
7
www.nature.com/scientificreports/ 33. Deng, S., Viola, L. & Ortiz, G. Majorana modes in timereversal invariant swave topological superconductors. Phys. Rev. Lett. 108, 036803 (2012). 34. Wang, J., Xu, Y. & Zhang, S.C. Twodimensional timereversalinvariant topological superconductivity in a doped quantum spinhall insulator. Phys. Rev. B 90, 054503 (2014). 35. Keselman, A., Fu, L., Stern, A. & Berg, E. Inducing timereversalinvariant topological superconductivity and fermion parity pumping in quantum wires. Phys. Rev. Lett. 111, 116402 (2013). 36. Gaidamauskas, E., Paaske, J. & Flensberg, K. Majorana bound states in twochannel timereversalsymmetric nanowire systems. Phys. Rev. Lett. 112, 126402 (2014). 37. Klinovaja, J. & Loss, D. Timereversal invariant parafermions in interacting rashba nanowires. Phys. Rev. B 90, 045118 (2014). 38. Danon, J. & Flensberg, K. Interaction effects on proximityinduced superconductivity in semiconducting nanowires. Phys. Rev. B 91, 165425 (2015). 39. Ebisu, H., Lu, B., Klinovaja, J. & Tanaka, Y. Theory of timereversal topological superconductivity in double rashba wires: symmetries of cooper pairs and andreev bound states. Prog. Theor. Exp. Phys. 2016, 083I01 (2016). 40. Klinovaja, J., Yacoby, A. & Loss, D. Kramers pairs of majorana fermions and parafermions in fractional topological insulators. Phys. Rev. B 90, 155447 (2014). 41. Sun, K., Chiu, C.K., Hung, H.H. & Wu, J. Tuning between singlet, triplet, and mixed pairing states in an extended hubbard chain. Phys. Rev. B 89, 104519 (2014). 42. Liu, C.X. & Trauzettel, B. Helical diracmajorana interferometer in a superconductor/topological insulator sandwich structure. Phys. Rev. B 83, 220510 (2011). 43. Schrade, C., Zyuzin, A. A., Klinovaja, J. & Loss, D. Proximityinduced p josephson junctions in topological insulators and kramers pairs of majorana fermions. Phys. Rev. Lett. 115, 237001 (2015). 44. Nakosai, S., Tanaka, Y. & Nagaosa, N. Topological superconductivity in bilayer rashba system. Phys. Rev. Lett. 108, 147003 (2012). 45. Zhang, Y. et al. Crossover of the threedimensional topological insulator bi2se3 to the twodimensional limit. Nature Phys. 6, 584–588 (2010). 46. Xu, S.Y. et al. Momentumspace imaging of cooper pairing in a halfdiracgas topological superconductor. Nature Phys. 10, 943–950 (2014). 47. Wray, L. A. et al. Observation of topological order in a superconducting doped topological insulator. Nature Phys. 6, 855–859 (2010). 48. Hor, Y. S. et al. Superconductivity in cuxbi2se3 and its implications for pairing in the undoped topological insulator. Phys. Rev. Lett. 104, 057001 (2010). 49. Kriener, M., Segawa, K., Ren, Z., Sasaki, S. & Ando, Y. Bulk superconducting phase with a full energy gap in the doped topological insulator cuxbi2se3. Phys. Rev. Lett. 106, 127004 (2011). 50. Sasaki, S. et al. Topological superconductivity in cuxbi2se3. Phys. Rev. Lett. 107, 217001 (2011). 51. Peng, H., De, D., Lv, B., Wei, F. & Chu, C.W. Absence of zeroenergy surface bound states in cuxbi2se3 studied via andreev reflection spectroscopy. Phys. Rev. B 88, 024515 (2013). 52. Matano, K., Kriener, M., Segawa, K., Ando, Y. & Zheng, G.q Spinrotation symmetry breaking in the superconducting state of cuxbi2se3. Nature Phys. 12, 852–854 (2016). 53. Yonezawa, S. et al. Thermodynamic evidence for nematic superconductivity in cuxbi2se3. Nature Phys. 13, 123–126 (2016). 54. Deutscher, G. & Feinberg, D. Coupling superconductingferromagnetic point contacts by andreev reflections. Appl. Phys. Lett. 76, 487–489 (2000). 55. Sato, K., Loss, D. & Tserkovnyak, Y. Crossed andreev reflection in quantum wires with strong spinorbit interaction. Phys. Rev. B 85, 235433 (2012). 56. Parhizgar, F. & BlackSchaffer, A. M. Unconventional proximityinduced superconductivity in bilayer systems. Phys. Rev. B 90, 184517 (2014). 57. Lu, H.Z., Shan, W.Y., Yao, W., Niu, Q. & Shen, S.Q. Massive dirac fermions and spin physics in an ultrathin film of topological insulator. Phys. Rev. B 81, 115407 (2010). 58. Shan, W.Y., Lu, H.Z. & Shen, S.Q. Effective continuous model for surface states and thin films of threedimensional topological insulators. New J. Phys. 12, 043048 (2010). 59. Fu, L. & Berg, E. Oddparity topological superconductors: Theory and application to cuxbi2se3. Phys. Rev. Lett. 105, 097001 (2010). 60. Fu, L. Oddparity topological superconductor with nematic order: Application to cuxbi2se3. Phys. Rev. B 90, 100509 (2014). 61. Anderson, P. Theory of dirty superconductors. J. Phys. Chem. Solids 11, 26–30 (1959). 62. Levy, N. et al. Experimental evidence for swave pairing symmetry in superconducting cuxbi2se3 single crystals using a scanning tunneling microscope. Phys. Rev. Lett. 110, 117001 (2013). 63. Qi, X.L., Hughes, T. L. & Zhang, S.C. Topological invariants for the fermi surface of a timereversalinvariant superconductor. Phys. Rev. B 81, 134508 (2010). 64. Haim, A., Wölms, K., Berg, E., Oreg, Y. & Flensberg, K. Interactiondriven topological superconductivity in one dimension. Phys. Rev. B 94, 115124 (2016). 65. Haim, A., Keselman, A., Berg, E. & Oreg, Y. Timereversalinvariant topological superconductivity induced by repulsive interactions in quantum wires. Phys. Rev. B 89, 220504 (2014). 66. Gangadharaiah, S., Braunecker, B., Simon, P. & Loss, D. Majorana edge states in interacting onedimensional systems. Phys. Rev. Lett. 107, 036801 (2011). 67. Stoudenmire, E. M., Alicea, J., Starykh, O. A. & Fisher, M. P. Interaction effects in topological superconducting wires supporting majorana fermions. Phys. Rev. B 84, 014503 (2011). 68. Recher, P. & Loss, D. Superconductor coupled to two luttinger liquids as an entangler for electron spins. Phys. Rev. B 65, 165327 (2002). 69. Hosseini, M. V. & Zareyan, M. Model of an exotic chiral superconducting phase in a graphene bilayer. Phys. Rev. Lett. 108, 147001 (2012). 70. Parhizgar, F. & Asgari, R. Magnetoresistance of a doublelayer hybrid system in a tilted magnetic field. Phys. Rev. B 90, 035438 (2014). 71. Yip, S.K. Models of superconducting cu:bi2se3: Single versus twoband description. Phys. Rev. B 87, 104505 (2013). 72. Wang, J. Electrically tunable topological superconductivity and majorana fermions in two dimensions. Phys. Rev. B 94, 214502 (2016).
Acknowledgements
The authors thank A. Bouhon, K. Björnson, and D. Kuzmanovski for discussions. This work was supported by the Swedish Research Council (Vetenskapsrå det), the Göran Gustafsson Foundation, the Swedish Foundation for Strategic Research (SSF), and the Wallenberg Academy Fellows program.
Author Contributions
A.B.S. proposed the idea and F.P. performed the calculations. Both authors analyzed the results and wrote the article. Scientific REPOrTS  7: 9817  DOI:10.1038/s4159801710510y
8
www.nature.com/scientificreports/
Additional Information
Competing Interests: The authors declare that they have no competing interests. Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations. Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/. © The Author(s) 2017
Scientific REPOrTS  7: 9817  DOI:10.1038/s4159801710510y
9